Download presentation

Presentation is loading. Please wait.

Published byPeyton Biss Modified over 3 years ago

1
FROM MESOSCALE SIMULATIONS TO MULTISCALE MODELLING Discrete Dislocation Plasticity Cambridge, 1-2 July 2004 L. Kubin &, B. Devincre LEM, CNRS-ONERA, F-Châtillon T. Hoc Ecole Centrale Paris, F-Châtenay Malabry R. Madec DPTA, CEA, F-Bruyères-Le-Châtel polycrystal continuum framework electronic scale dislocation core properties microstructure single crystal dislocation core dislocation: elastic properties atomic scale

2
OUTLINE 1 DDD simulations elastic properties 2DDD simulations connection with atomic scale 3Typical problems at mesoscale 4Coupling with the continuum Full DDD Constitutive modelling Continuum theory of dislocations ?

3
interactions P-K force line tension junctions mobility laws cross-slip............ (2-D, 2.5-D) 3-D SIMULATIONS dislocation flux (basic DDD) + stress equilibrium (full DDD) 3 = (Periodic) boundary conditions 1 = Elastic properties 2 = Local rules Discretisation time (10 -9 - 10 -10 s) & space line & character 10 -15 m FCC, BCC, HCP, DC..

4
Elastic properties of dislocations can be very complicated not an issue for DDDs down to a few Burgers vectors dislocations vs. small loops, other dislocations, obstacles (planar glide)

5
DISLOCATIONS AND DEFECT CLUSTERS (radiation damage & fatigue) Drift mechanism Kratochvil 1986 Sweeping mechanism Sharp-Makin 1964.... Ghoniem et al. b Atomistic vision: the cluster is absorbed (Rodney & Martin 1999)

6
JUNCTIONS -> FOREST HARDENING D. Rodney & R. PHillips, 2000 (MS) R. Madec et al. 2001 The Lomer-Cottrell lock (Saada 1960, Schoeck & Frydman 1972) ≈ same critical stresses ( b/ ) junctions ≈ elastic problem => no free parameter

7
STRENGTH OF THE FOREST CuAlCu & Ag (Basinski, 1979) DD Up to large strains, ≈ insensitive to: SFE, Cross-slip, rotations, long range stresses, GNDs, & patterning fccs: 0.35 ±0.15

8
Local rules

9
series connection with atomic scale needs models : rate equations, elastic models (Escaig, Schoeck et al.,..) => saddle points, equilibrium (MS simulations) fast events (MD simulations) Dislocation theory is not finished.... FCCs : cross-slip (Cu) & scaling laws BCCs : ab initio core structure (C. Woodward) kink-pair mechanism (J. Moriarty) * solute atoms and screw dislocation cores (BCCs, Ti) * dislocation generation in defect-free volumes - homogeneous (S. Yip) - heterogeneous (crack tips, surfaces, nanoindentation, grain boundaries, interphases, epitaxial layers..) LOCAL RULES

10
MOBILITY / MICROSTRUCTURE b = Bv; v << v Obstacle : d-d interactions (athermal) FCCs : Patterning √ Thermally activated obstacle: the lattice No pattern v = v o Exp[- G( )]/kT.. up to medium-high temperature or large strains ≠ √ Nb 50K fast moving dislocations (Zbib et al.), climb velocities ?

11
CROSS-SLIP (FCCs): MESOSCOPIC VIEW multiplication/annihilation dynamic recovery pattern formation precipitate bypassing textures Local rule : P exp[- G( *, )/kT) Friedel-Escaig elastic model atomistic models -> Jacobsen et al(1997..) Rao et al. (1999) seen in literature: P = 0 (planar slip), P = 1(perfect screws) b b

12
MESOSCOPIC LOCAL RULES dissociation : attractive stress between the partials precipitate: glide resistance inside the precipitate (shearing) grain boundary/interface: dislocations are blocked, absorbed (re-emitted), cross ?..... mesoscale simulations are weak in chemistry

13
Typical issues for basic DDDs single crystal: hardening & patterning interactions between slip systems composition of mechanisms (ex: Peierls stress + forest hardening)

14
MASS SIMULATIONS Cu, [100] stress axis. Not necessarily the best way for understanding hardening

15
CELLS and CROSS-SLIP (111) foil t = 3 m 10 m von Mises stress (110) foil t = 3 m "similitude principle" ? structure of internal stress

16
Interactions between slip systems

17
INTERACTION COEFFICIENTS (FCCs) a 0: : self a 1copla : coplanar junctions a 3 : Lomer a 2 : glissile a 1ortho : Hirth + the collinear interaction(b SP, b CSP): a coli measurement by model simulations: a coli ≈ 15 a 3 c = b√ (Franciosi et al., 1980) 12x12 = 144 => 6

18
THE COLLINEAR INTERACTION P1 ≠ P2 same b exhausts the mobile dislocations leaves small stable debris

19
COLLINEAR INTERACTIONS SiGe/Si: (after Stach et al., 2000) Al-6Mg in situ (Mills)

20
STRESS-STRAIN CURVES IN MULTISLIP Cu, 300 K, [100], 8 active slip systems DD simulation critical stresses reconstructed from A : the cross-slip systems of B remain active A', B' same but without collinear interaction B: 4 slip systems are de-activated

21
Coupling with the continuum : full DDD

22
NANO-GRAINS d (nm -1/2 ) Cu J. Weertman 1997 Ni d (nm) d -1/2 Atomistic simulations: d ≈ 30-50 nm but still no Hall-Petch law ! DDD simulations ?

23
HALL-PETCH scaling k ?(atomic ? meso ?) dislocation-grain boundary (local rule at mesoscale) continuum modelling ? 1 - pile-ups d N disl d joint N disl d k/√d (yield ) +k /d (flow) ==> 2 - storage 3 - GNDs

24
3D MMC COMPOSITE (full DDD) (001 view) S. Groh 2003 7 m There are size effects in 001 and density/stress gradients but: how can we compose mechanisms : forest hardening (basic DDD) + load transfer (FE) + size effects (full DDD) ?

25
CONSTITUTIVE MODELLING Basic DDD simulations are used to feed (tensorial) dislocation-based constitutive models Avoids/limits parameter fitting Many possible applications up to large strains = atomic + meso + continuum Basic DDD + dislocation-based models + crystal plasticity codes

26
HARDENING MATRIX cf. Kocks-Mecking Teodosiu et al. (Franciosi, 1980) storage recovery Forest densities only, no space variable interaction coefficients (measured by DDD) critical annihilation distance (cross-slip models) mean-free path (from experiment) This constitutive formulation is parameter-free for copper crystals It is inserted into a crystal plasticity FE code (boundary conditions..)

27
Cu crystals (Diehl, 1956) [531] (MPa) "Al": y s = 500 nm Cu: y s = 50 nm "Ag": y s = 12 nm (T. Takeuchi, 1974) l/l o F/S o (MPa) [001] 4 active slip systems instead of 8

28
STAGE I - STAGE II (MPa) No information needed about dislocation structures as long as there is no change in deformation path Next step: Bauschinger test Prediction of slip systems

29
STRAIN LOCALIZATIONS: JERKY FLOW FE code for polycrystals (A. Beaudoin): no gradient term, incompatibity stresses Constitutive formulation: Al-Mg alloy 2 10 -4 s -1 Type B All types of bands and dynamic behaviour = F( ) S. Kok et al. Acta Mater. 51 (2003) 3651

30
CONTINUUM THEORY OF DISLOCATIONS ? A. El Azab (2000..) finite crystal distortions elastic fields dislocation structure statistical dislocation dynamics framework, 3D, accounts for all reactions ≈ analytical version of a full DDD simulation complex (≈ 60 equations) goes to large strains

31
SUMMARY All DDDs: local rules (need atomistic input) small strains Basic DDD : tool for modelling/understanding interactions, microstructures, strain hardening more powerful, modelling & connection with crystal plasticity codes Fulll DDD : applications:...potentially,almost everything small strains few achievements till now (in 3-D) can we draw models from it ?

Similar presentations

OK

ASE324: Aerospace Materials Laboratory Instructor: Rui Huang Dept of Aerospace Engineering and Engineering Mechanics The University of Texas at Austin.

ASE324: Aerospace Materials Laboratory Instructor: Rui Huang Dept of Aerospace Engineering and Engineering Mechanics The University of Texas at Austin.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on crash fire tender Ppt on all types of motion Ppt on abstract artwork Ppt on eisenmenger syndrome vsd Ppt on birds and animals Reproductive system anatomy and physiology ppt on cells Ppt on electric arc furnace Ppt on revolt of 1857 pictures Ppt on metrics in software project management Ppt on event driven programming wiki